세계 제일의 방대한 재료 데이터베이스

# Linear Elastic Fracture Mechanics : Part One

요약:

The theory of Linear Elastic Fracture Mechanics (LEFM) has been developed using a stress intensity factor (K) determined by the stress analysis, and expressed as a function of stress and crack size.

The elements of fracture mechanics may be summarized in the form of a triangle having the 3 critical parameters situated at each apex: working stress, fracture toughness and critical flaw size. If two of the three parameters are known, the third can be calculated...

### INTRODUCTION

For decades, fracture mechanics has been used to study the fatigue crack propagation of mechanical components. Great efforts have been made to investigate the growth rate and mechanism of the fatigue crack in different conditions. Many of the studies focused on establishing a method using a few clear parameters to describe the fatigue crack growth rate.

Linear Elastic Fracture Mechanics (LEFM) is the basic theory of fracture, originally developed by Griffith (1921 to1924) and completed in its essential form by Irwin (1957, 1958) and Rice (1968 a,b). LEFM is a highly simplified, yet sophisticated, theory that deals with sharp cracks in elastic bodies.

LEFM is applicable to any material as long as certain conditions are met. These conditions rely on the presence of all basic ideal conditions analyzed in LEFM in which all materials are elastic except in a vanishingly small region (a point) at the crack tip. In fact, the stress near the crack tip is so high that some kind of inelasticity must take place in the immediate vicinity of the crack tip.

However, if the size of the inelastic zone is small relative to the linear dimensions of the body (including the size of the crack itself), then the disturbance introduced by this small inelastic region is also small. Therefore LEFM and point of failure can be verified exactly. Using this information LEFM theory can therefore be used as the basic foundation for the behavior of any material prone to cracking (such as concrete) even though precise LEFM calculations cannot be made.

The theory of Linear Elastic Fracture Mechanics (LEFM) has been developed using a stress intensity factor (K) determined by the stress analysis, and expressed as a function of stress and crack size i.e. (stress) x (length)1/2. The strain energy release rate, or the stress intensity at the crack tip (KC), eventually, will inevitably reach a critical value.

There are three modes of fracture, Mode I being identified as the opening mode, in which the crack surfaces move opposite and perpendicular to each other (as when opening by driving in a wedge).This mode is the most important from the low stress fracture point of view and has been studied more extensively than modes II and III, which involve sliding and lateral tearing respectively. The basic assumption is that crack propagation will occur when the strain energy release rate, or the stress intensity at the crack tip KC reaches a critical value. As previously mentioned, mode I is the most important when considering the low stress fracture.

Plane strain is defined as a state of two dimensional strain, i.e. there is no strain in the through-thickness direction, and is therefore classed as a state of triaxial stress. The ideal conditions of stress are not usually realized in practice and a mixed mode state of stress exists. Even in very brittle fractures, some plastic flow may occur at the tip of a sharp defect.

In order to establish the critical stress intensity by Linear Elastic Fracture Mechanics, the plastic zone must be kept small in comparison to the other dimensions of the specimen. For what is essentially plane strain conditions, the inherent fracture toughness of a material can be expressed in terms of the critical value of the stress intensity factor KIC at which crack instability occurs. The value of KIC has to be determined experimentally but, once properly determined under one set of conditions, it is equally applicable to other conditions.

The value of KIC does, of course, vary markedly with metallurgical variables, such as steelmaking practice and inclusions, and heat treatment and microstructure, but it can be used to compare steels of different strength levels by use of the same parameter, which is not possible when using alternative approaches, such as those based on transition temperature.

The elements of fracture mechanics may be summarized in the form of a triangle having the 3 critical parameters situated at each apex: working stress (σw), fracture toughness (KIC) and critical flaw size (acrit). If two of the three parameters are known, the third can be calculated; this simple concept emphasizes the importance of being able to accurately measure the size of the discontinuity.

Furthermore, the exact magnitude and distribution of the stresses in a component may not be known and therefore, it is obvious why a safety factor has to be applied. But residual stresses in a casting can be of a surprisingly high order before the working stress is applied. Consequently, some knowledge of the magnitude of possible residual stress is essential.

## 기술 자료 검색

검색할 어구를 입력하십시오:

 검색 범위 본문 키워드 머릿글 요약

 이 문서는 전체 문서 중 일부분입니다. 이 주제에 대해 더 읽고 싶으시면 아래 링크를 클릭하시면 됩니다.

Total Materia Extended Range는 수천개 금속 합금의 열처리 조건 및 하중 조건에 대한 파괴 공학 변수 데이터베이스를 포함하고 있습니다. K1C, KC, 균열 성장 및 Paris 법칙 변수와 이에 대응되는 균열 성장 그래프가 제공됩니다.

단조 특성도 참조를 위해 추가되어 있으며 단조 특성을 통해 예상되는 빠진 변수의 추정치도 필요한 곳에는 포함되어 있습니다.

신속 검색에 검색할 재질명을 입력합니다. 원하신다면 국가/규격을 지정하신 후 검색 버튼을 클릭합니다.

결과 리스트에서 재질을 선택하시면, 일련의 규격 사양 소그룹이 나타납니다.

Total Materia 파괴 공학 데이터는 규격 사양서와 무관하므로, 어떠한 소그룹 내의 링크를 클릭하셔도 파괴 공학 데이터를 검토하실 수 있습니다.

데이터는 표로 출력되며, 가능한 곳에는 Paris 곡선(Region II)와 함께 출력되어 있습니다. 데이터 출처에 관한 정확한 참조가 각 데이터에 주어져 있습니다.

Total Materia 데이터베이스를 사용해 보실 수 있는 기회가 있습니다. 저희는 Total Materia 무료 체험을 통해 150,000명 이상의 사용자가 이용하고 있는 커뮤니티로 귀하를 초대합니다.